Luminescence properties of silicon-cellulose nanocomposite
© Pikulev et al.; licensee Springer. 2012
Received: 30 April 2012
Accepted: 19 July 2012
Published: 31 July 2012
We have characterized the structure and luminescence properties for two-component material composed of nanocrystalline cellulose and nanocrystalline (less to 100 nm) silicon powder. An efficient and stable photoluminescence of nanocomposite, resistant to the influence of gas-phase oxidants, has been found. The obtained material has electret-like properties and demonstrates the possibility of multiple-recharging in an electric field near 5·103 V/cm at temperatures ranging from −70°C to 100°C. The presence of the electric field, as well as ozone or low-temperature plasma treatment, does not change the luminescence spectrum due to quantum size properties of silicon nanoparticles. We believe that these particles may appear in two states: both embedded in a cellulose matrix and in the form of mechanical mixture.
KeywordsNanosilicon Porous silicon Nanocellulose Photoluminescence Electret
Luminescence properties of porous silicon or nanosilicon powder are severely degraded by the influence of gas-core oxidants (like O2, O3, and NO2) via oxidation of silicon nanoparticles [1, 2]. To stabilize the photoluminescence (PL) activity of silicon nanoparticles, they are to be placed in an optically transparent medium (such as silica and polymer films). In the current case, the problem was solved by the introduction of silicon nanoparticles into a matrix of cellulose macromolecules. Despite the fact that polymer macromolecules synthesis with metal nanoparticles is rather thoroughly investigated , the studies of physical properties of silicon nanoparticles in natural polymers are poorly represented in scientific literature. We were able to find one paper  revealing phenomenon which is close to the current topic. In the above-mentioned work, the luminescent properties of ethyl cellulose nanoparticles containing embedded semiconductor nanocrystals have been investigated. Since only the general model of the luminescence mechanism was suggested by the author, the issue of the excitation transfer between the semiconductor nanoparticles and fragments of organic molecules is still under discussion. On the contrary, we are focused on the PL of silicon nanocrystals  in the solid-state media, since there is no generally accepted hypothesis to explain the phosphorescence of pure cellulose-I (without lignins) under ultraviolet (UV) excitation .
On the other hand, our choice of the matrix for the silicon nanoparticles injections is caused by the fact that cellulose is the most widespread and naturally renewable polymer. The development of environmentally friendly ‘paper electronics’ may bring the cost reduction in comparison with functional analogs of silicon electronics devices in the future. There is a reference for two papers: one of them describes the development of organic light-emitting diode based on luminescent cellulose  and the other presents the first ‘paper transistor’ on a carbon nanotube . Currently, the technology of improvement of the physical properties of tissue (fire-resistant, in the first place) with silica nanoparticles is carried out into the industrial level of production . We obtained the nanocomposite material which can be used currently as a hidden marker for identification of papers, showing stable luminescence properties under UV irradiation.
There were three stages in the process of nanocomposite preparation. The method of preparation of nanocrystalline cellulose (NCC), which is based on a modification of chemically pure microcrystalline cellulose (MCC), pre-milled in an agate mortar in aqueous solution of 38% hydrochloric and 98% sulfuric acids (1:3:6 distilled water resp.) with periodic ultrasonic dispersion of mixture during several hours was used in the first stage of the experiment. The acidity of the solution was increased up to pH 3 by repeated dilution with distilled water. A similar method proposed in  allowed the authors to obtain particles of crystalline cellulose with diameter in the range from 20 to 100 nm (the results of transmission electron microscopy). In the current case, the value of the average size of a cellulose particle in suspension made up more than 60 nm, even after the separation of the heavy fraction of the suspension. This result can be explained by fast coagulation of the cellulose particles in the solutions. For further studies, we took samples from the upper (NCC-1) and lower (NCC-2) parts of the suspension which were subjected to partial sedimentation.
The second stage of the process consists of the preparation of nanocrystalline silicon. The source of silicon nanocrystals was porous silicon. For the preparation of porous Si, we used a standard electrochemical etching of p-Si wafer (100), 1 Ω·cm in 40% HF and isopropanol (1:1) solution by constant current density 50 mA/cm2 by visible light illumination. The suspension of particles of nanocrystalline silicon was formed in isopropanol solution by mechanical destruction of porous silicon sample placed in the solution. The silicon particles in the solution were subjected to subsequent ultrasonic dispersion of the colloidal solution for 30 min; as a result, the sizes of silicon particles in solution got distributed in the range from a few to 100 nm. In addition, a nonluminous Si powder, prepared by plasmachemical decomposition of monosilane in Ar plasma in an inductive discharge, was used.
The last stage consisted of mixing nanocellulose and Si nanoparticles in water-alcohol or pure alcohol solution by ultrasonic dispersion, evaporation, and molding by 0.26 MPa pressure. As a result a 0.2-mm thickness beige-colored tablet of nanocomposite with stable PL activity was obtained.
The X-ray investigations (X-ray diffraction, XRD) were performed on DRON-6.0 diffractometer (Bourevestnik, Inc., St. Petersburg, Russia) using CuKα-radiation. The degree of crystallinity of the original and the synthesized samples was carried out by X-ray data . To obtain the infrared absorption spectra, the FT-801 Fourier transform infrared spectroscopy (FTIR) spectrometer (Simex, Inc., Novosibirsk, Russia) with nitrogen-cooled mercury cadmium telluride detector has been used. For the PL excitation we applied the 15 mW He-Cd laser.
Results and discussion
There are weak peaks from the crystalline phase of silicon Si (Joint Committee on Powder Diffraction Standards - International Centre for Diffraction Data, JCPDS card 5–565) on X-ray diffraction pattern (Figure 1b). Since the amount of the amorphous phase in the first series of nanocomposite increases by 20% compared with the original NCC-1, we assume that during the synthesis of new material, a certain amount of silicon nanoparticles embedded in the cellulose matrix, and the rest formed mechanical mixture with it. In the second series of the composite, no increase on the amount of amorphous phase was observed. Thus, we conclude that the use of NCC with a lower degree of crystallinity makes possible a penetration the silicon nanoparticles in a polymer matrix without changing its structure.
The PL spectrum of nanocomposite (Figure 3, curve 4 a) shows more effective luminescence than as-prepared porous Si (curve 1 a) with an equal amount of nanomaterial. Curve 2 refers to PL of MCC sample. The shape of this spectrum in some cases split into several peaks, indicating the presence of few types of organic fluorophores in a matrix of cellulose. A possible reason for such luminescence might be the presence of carbonyl groups and different kinds of low-molecular products of cellulose destruction in this material . After the formation of NCC, a fluorescent activity in short-wavelength region is significantly reduced (curve 3), and in the case of nanocomposite practically disappears (curve 4). In this case, the presence of Si nanoparticles leads to the suppression of short-wave emission, but it is premature to assume the existence of an energy transfer channel from cellulose matrix to semiconductor nanoparticles.
When a nanocomposite was heated in air, its PL properties were practically unchanged up to 100°C. Above this temperature the carbonization of the NCC begins, and the PL intensity greatly decreases. This fact is also consistent with the destruction of hydrogen passivation on the surface of nanocrystals due to breakdown of the cellulose molecules. Also note that dissolving of tablets in water and re-pressing remains the luminescent activity on the same level.
Our presented results demonstrate a preparation method and specific PL and electrical properties of new ‘silicon-cellulose’ nanocomposite. In this case high retention of PL properties under external influences is determined for the ranges of chemical stability of cellulose molecules. The effects of temperature, gas-phase oxidation, and low-temperature plasma treatment show high stability of the PL properties of the composite. We have discussed a stabilization mechanism of the luminescent properties of nanocomposite, as well as the possibility of energy and charge transfer between the nanoparticles of silicon and cellulose.
Fourier transform infrared spectroscopy
We would like to thank Dr. Valery A. Gostev for providing a micro-plasmatron and advice on experiments with low-temperature plasma. Studies were carried out in the framework of the Russian Federal Targeted Program ‘Scientific and pedagogical personnel of innovative Russia’, project number 14.740.11.0018.
- Cullis AG, Canham LT, Calcott PDJ: The structural and luminescence properties of porous silicon. Appl Phys Rev 1997, 82(3):909. 10.1063/1.366536View ArticleGoogle Scholar
- Pikulev V, Tsyganenko A, Kuznetsov S, Saren A, Gurtov V: Peculiarities of ozone adsorption on a porous silicon surface at low temperature. Phys Stat Sol C 2007, 4: 2116. 10.1002/pssc.200674394View ArticleGoogle Scholar
- Pomogailo AD, Kestelman VN: Metallopolymer Nanocomposites. Springer, Heidelberg; 2005.Google Scholar
- Generalova AN, Sizova SV, Oleinikov VA, Zubov VP, Artemyev MV, Spernath L, Kamyshny A, Magdassi S: Highly fluorescent ethyl cellulose nanoparticles containing embedded semiconductor nanocrystals. Colloids and Surfaces A 2009, 342: 59. 10.1016/j.colsurfa.2009.04.007View ArticleGoogle Scholar
- Kumar V: Nanosilicon. Elsevier, Oxford; 2007.Google Scholar
- Tylli H, Forsskåhl I, Olkkonen C: The effect of heat and IR radiation on the fluorescence of cellulose. Cellulose 2000, 7: 133. 10.1023/A:1009225624732View ArticleGoogle Scholar
- Karakawa M, Chikamatsu M, Nakamoto C, Maeda Y, Kubota S, Yase K: Organic light-emitting diode application of fluorescent cellulose as a natural polymer. Macromol Chem Phys 2007, 208(18):2000. 10.1002/macp.200700154View ArticleGoogle Scholar
- Yun S, Jang SD, Yun GY, Kim JH, Kim J: Paper transistor made with covalently bonded multiwalled carbon nanotube and cellulose. Appl Phys Lett 2009, 95: 104102. 10.1063/1.3224200View ArticleGoogle Scholar
- Mahltig B, Textor T: Nanosols and Textiles. World Scientific, Toh Tuck Link; 2008.View ArticleGoogle Scholar
- Wang N, Ding E, Cheng R: Preparation and liquid crystalline properties of spherical cellulose. Langmuir 2008, 24: 5. 10.1021/la702923wView ArticleGoogle Scholar
- Rabek JF: Experimental Methods in Polymer Chemistry. Wiley, New York; 1980.Google Scholar
- Zugenmaier P: Crystalline Cellulose and Derivatives: Characterization and Structures. Springer, Heidelberg; 2008.View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.